# diffusion - how do atoms move through solids? diffusion

Post on 20-Dec-2016

217 views

Embed Size (px)

TRANSCRIPT

1MSE 2090: Introduction to Materials Science Chapter 5, Diffusion

Diffusion - how do atoms move through solids?

Diffusion mechanismsVacancy diffusion Interstitial diffusionImpurities

The mathematics of diffusionSteady-state diffusion (Ficks first law)Nonsteady-State Diffusion (Ficks second law)

Factors that influence diffusionDiffusing speciesHost solidTemperatureMicrostructure

Chapter Outline

2MSE 2090: Introduction to Materials Science Chapter 5, Diffusion

Diffusion is material transport by atomic motion.

Inhomogeneous materials can become homogeneous by diffusion. For an active diffusion to occur, the temperature should be high enough to overcome energy barriers to atomic motion.

What is diffusion?

results of an atomistic simulation of atomic mixinghomework project in MSE 4592/6270

3MSE 2090: Introduction to Materials Science Chapter 5, Diffusion

Interdiffusion (or impurity diffusion) occurs in response to a concentration gradient.

Self-diffusion is diffusion in one-component material, when all atoms that exchange positions are of the same type.

Interdiffusion and Self-diffusion

Before After

(Heat)

4MSE 2090: Introduction to Materials Science Chapter 5, Diffusion

Vacancy diffusion mechanism

To jump from lattice site to lattice site, atoms need energy to break bonds with neighbors, and to cause the necessary lattice distortions during jump. This energy comes from the thermal energy of atomic vibrations (Eav ~ kBT)

The direction of flow of atoms is opposite the vacancy flow direction.

Diffusion Mechanisms (I)

Atom migration Vacancy migration

AfterBefore

5MSE 2090: Introduction to Materials Science Chapter 5, Diffusion

Interstitial diffusion mechanism

Diffusion Mechanisms (II)

Interstitial atom before jump

Interstitial atom after jump

Interstitial diffusion is generally faster than vacancy diffusion because bonding of interstitials to the surrounding atoms is normally weaker and there are many more interstitial sites than vacancy sites to jump to.

Requires small impurity atoms (e.g. C, H, O) to fit into interstices in host.

6MSE 2090: Introduction to Materials Science Chapter 5, Diffusion

The flux of diffusing atoms, J, is used to quantify how fast diffusion occurs. The flux is defined as either the number of atoms diffusing through unit area per unit time (atoms/m2-second) or the mass of atoms diffusing through unit area per unit time, (kg/m2-second).For example, for the mass flux we can write

Diffusion Flux

J = M / At (1/A) (dM/dt) (Kg m-2 s-1)

where M is the mass of atoms diffusing through the area A during time t.

AJ

7MSE 2090: Introduction to Materials Science Chapter 5, Diffusion

Steady state diffusion: the diffusion flux does not change with time.

Concentration profile: concentration of atoms/molecules of interest as function of position in the sample.

Concentration gradient: dC/dx (Kg m-4): the slope at a particular point on concentration profile.

Steady-State Diffusion

BA

BA

xxCC

xC

dxdC

=

8MSE 2090: Introduction to Materials Science Chapter 5, Diffusion

Ficks first law: the diffusion flux along direction x is proportional to the concentration gradient

Steady-State Diffusion: Ficks first law

where D is the diffusion coefficientdxdCDJ =

The concentration gradient is often called the driving forcein diffusion (but it is not a force in the mechanistic sense).The minus sign in the equation means that diffusion is down the concentration gradient.

9MSE 2090: Introduction to Materials Science Chapter 5, Diffusion

Why do the random jumps of atoms result in a flux of atoms from regions of high concentration towards the

regions of low concentration?

Diffusion down the concentration gradient

Atoms here jump randomly both right and left

But there are not many atoms here to jump to the left

As a result there is a net flux of atoms from left to right.

dxdCDJ =

10MSE 2090: Introduction to Materials Science Chapter 5, Diffusion

In many real situations the concentration profile and the concentration gradient are changing with time. The changes of the concentration profile can be described in this case by a differential equation, Ficks second law.

Nonsteady-State Diffusion: Ficks second law

Solution of this equation is concentration profile as function of time, C(x,t):

2

2

xCD

xCD

xtC

=

=

11MSE 2090: Introduction to Materials Science Chapter 5, Diffusion

Nonsteady-State Diffusion: Ficks second law

2

2

xCD

tC

=

Ficks second law relates the rate of change of composition with time to the curvature of the concentration profile:

Concentration increases with time in those parts of the system where concentration profile has a positive curvature. And decreases where curvature is negative.

C

x

C

x

C

x

The phenomenological description based on the Fickslaws is valid for any atomic mechanism of diffusion. Understanding of the atomic mechanisms is important, however, for predicting the dependence of the atomic mobility (and, therefore, diffusion coefficient) on the type of interatomic bonding, temperature, and microstructure.

12MSE 2090: Introduction to Materials Science Chapter 5, Diffusion

To jump from lattice site to lattice site, atoms need energy to break bonds with neighbors, and to cause the necessary lattice distortions during jump. The energy necessary for motion, Em, is called the activation energy for vacancy motion.

Diffusion Thermally Activated Process (I) (not tested)

Schematic representation of the diffusion of an atom from its original position into a vacant lattice site. Activation energy Em has to be supplied to the atom so that it could break inter-atomic bonds and to move into the new position.

AtomVacancyEm

Distance

Ener

gy

13MSE 2090: Introduction to Materials Science Chapter 5, Diffusion

The average thermal energy of an atom (kBT = 0.026 eVfor room temperature) is usually much smaller that the activation energy Em (~ 1 eV/atom) and a large fluctuation in energy (when the energy is pooled together in a small volume) is needed for a jump.

The probability of such fluctuation or frequency of jumps, Rj, depends exponentially on temperature and can be described by equation that is attributed to Swedish chemist Arrhenius:

Diffusion Thermally Activated Process (II) (not tested)

where R0 is so-called attempt frequency proportional to the frequency of atomic vibrations.

= Tk

EexpRRB

m0j

14MSE 2090: Introduction to Materials Science Chapter 5, Diffusion

For the vacancy diffusion mechanism the probability for any atom in a solid to move is the product of

the probability of finding a vacancy in an adjacent lattice site (see Chapter 4):

Diffusion Thermally Activated Process (III) (not tested)

The diffusion coefficient can be estimated as

= Tk

EexpRRB

m0j

= Tk

QzPB

vexp

=

Tk

QTk

EazRDB

V

B

m expexp20

( )

=

+= Tk

QexpDTkQEexpD

B

d0

B

Vm0

Temperature dependence of the diffusion coefficient, follows the Arrhenius dependence.

z is coordination number (number of atoms adjacent to the vacancy)

and the frequency of jumps (probability of thermal fluctuation needed to overcome the energy barrier for vacancy motion):

15MSE 2090: Introduction to Materials Science Chapter 5, Diffusion

Diffusion coefficient is the measure of mobility of diffusing species.

Diffusion Temperature Dependence (I)

The activation energy Qd and preexponential D0, therefore, can be estimated by plotting lnD versus 1/T or logDversus 1/T. Such plots are called Arrhenius plots.

= RT

QexpDD d0

dxdCDJ =

D0 temperature-independent preexponential (m2/s)Qd the activation energy for diffusion (J/mol or eV/atom)

R the gas constant (8.31 J/mol-K or 8.6210-5 eV/atom-K)T absolute temperature (K)

=

T1

RQDlnDln d0

=

T1

R3.2QDlogDlog d0or

The above equation can be rewritten as

16MSE 2090: Introduction to Materials Science Chapter 5, Diffusion

Diffusion Temperature Dependence (II)

Graph of log D vs. 1/T has slop of Qd/2.3R, intercept of log Do

=21

21d T1T1

DlogDlogR3.2Q

=

T1

R3.2QDlogDlog d0

baxy +=

0logDb =

2.3RQa d=

1/Tx =

17MSE 2090: Introduction to Materials Science Chapter 5, Diffusion

Temperature dependence: Interstitial and vacancy diffusion mechanisms (I)

Diffusion of interstitials is typically faster as compared to the vacancy diffusion mechanism (self-diffusion or diffusion of substitutional atoms).

=

T1

2.3RlogDlogD 0 d

Q

18MSE 2090: Introduction to Materials Science Chapter 5, Diffusion

=

TkQexpDD

B

d0

770.47N in BCC Fe

1450.34N in FCC Fe

430.63H in FCC Fe

150.12H in BCC Fe

871.1C in BCC Fe13823C in FCC FeQd, kJ/molD0, mm2/s-1Impurity

Smaller atoms cause less distortion of the lattice during migration and diffuse more readily than big ones (the atomic diameters decrease from C to N to H).

Diffusion is faster in open lattices or in open directions

242230Ni in Cu

460180000Si in Si

246410Fe